|Year : 2022 | Volume
| Issue : 1 | Page : 82
Effect of sintering temperature on translucency parameter of zirconia blocks
Fariborz Vafaei1, Armaghan Shahbazi2, Amirarsalan Hooshyarfard3, Amir Hosein Najafi4, Maziar Ebrahimi4, Maryam Farhadian5
1 Dental Implants Research Center, Department of Prosthodontics, Faculty of Dentistry, Hamadan University of Medical Sciences, Hamadan, Iran
2 Department of Prosthodontics, Faculty of Dentistry, Tehran Medical Sciences, Islamic Azad University, Tehran, Iran
3 Department of Periodontics, Dental Materials Research Center, Tehran Medical Sciences, Islamic Azad University, Faculty of Dentistry, Shahed University, Tehran, Iran
4 Dentist, Private Practice, Hamadan University of Medical Sciences, Hamadan, Iran
5 Department of Biostatistics, School of Public Health and Research Center for Health Sciences, Hamadan University of Medical Sciences, Hamadan, Iran
|Date of Submission||26-Dec-2020|
|Date of Acceptance||16-Apr-2022|
|Date of Web Publication||20-Oct-2022|
Dr. Armaghan Shahbazi
Department of Prosthodontics, Faculty of Dentistry, Tehran Medical Sciences, Islamic Azad University, Tehran
Source of Support: None, Conflict of Interest: None
Background: The main drawbacks of zirconia are its high refractive index and opacity. This study aimed to assess the effect of sintering temperature on the translucency of Ivoclar e. max ZirCAD (IEZ), and White Peaks Symphony (WPS) zirconia blocks.
Materials and Methods: In this in vitro experimental study, 30 IEZ and 30 WPS zirconia blocks measuring 10 mm × 10 mm × 1 mm were prepared and underwent sintering in three subgroups at 1440°C, 1500°C, and 1530°C. The specimens were then photographed against a black and a white background with a standard digital camera. The L*, a*, and b* color parameters were measured using Adobe Photoshop software, and translucency was calculated. Data were analyzed using one-way ANOVA and Tukey's test (P < 0.05).
Results: In both the IEZ and WPS groups, the maximum and minimum translucency parameters were recorded in 1530°C and 1440°C subgroups, respectively. The difference in the mean translucency was significant among the three subgroups of each zirconia group (P < 0.001). The mean translucency of WPS zirconia was significantly higher than that of IEZ zirconia (P < 0.01), and maximum difference was noted at 1500°C sintering temperature.
Conclusion: Increasing the sintering temperature from 1440°C to 1530°C can significantly increase the translucency of IEZ and WPS zirconia blocks, and can be considered to improve the quality of zirconia restorations.
Keywords: Ceramics, refractometry, yttria-stabilized tetragonal zirconia
|How to cite this article:|
Vafaei F, Shahbazi A, Hooshyarfard A, Najafi AH, Ebrahimi M, Farhadian M. Effect of sintering temperature on translucency parameter of zirconia blocks. Dent Res J 2022;19:82
|How to cite this URL:|
Vafaei F, Shahbazi A, Hooshyarfard A, Najafi AH, Ebrahimi M, Farhadian M. Effect of sintering temperature on translucency parameter of zirconia blocks. Dent Res J [serial online] 2022 [cited 2023 Apr 1];19:82. Available from: https://www.drjjournal.net/text.asp?2022/19/1/82/359319
| Introduction|| |
In the past decades, many attempts have been made to improve the quality of dental ceramics to better mimic the esthetic and mechanical properties of natural teeth., Resultantly, a wide variety of dental ceramics such as feldspathic, leucite, lithium disilicate, fluorapatite glass, zirconia, and mixed ceramics have been introduced to the market.,, Different types of all-ceramic and zirconia restorations are used in dentistry. As a general rule, a ceramic restoration should have excellent mechanical and esthetic properties resembling those of natural teeth.,, Monolithic zirconia restorations have gained increasing popularity in recent years due to their optimal color, causing minimal wear of the opposing teeth, conservative preparation design, and high long-term clinical success rate.,
Translucency is an important parameter that plays a fundamental role in creating a natural tooth color. Translucency refers to the property of passage of light through a material, and can be adjusted by controlling the amount of absorption, reflectance, scattering, and transmission of light., Low reflectance and high scattering and transmission of light increase translucency. Translucency can be measured by using different equations via different tools. The most commonly used parameter for the calculation of translucency is the color difference of an object with a uniform thickness against a black and a white background.
Sintering is a fundamental step in the preparation of prosthetic restorations, which can significantly affect their properties. In the process of zirconia sintering, heat is transferred from the surface to the core to obtain a mature zirconia. The sintering temperature is a critical parameter affecting the size and density of zirconia particles. It directly affects the density, porosity, and growth of zirconia particles., Zirconia, with a relative refractive index of 2.2, has the highest rate of porosities in the core among different ceramic materials. By decreasing these porosities and obtaining a denser material, the translucency of zirconia blocks can be improved, and a more favorable color can be achieved., Thus, dental clinicians can improve the optical properties of zirconia by changing its crystalline structure via adjusting the sintering conditions.
The available studies on the effect of sintering temperature on the translucency of different types of zirconia have reported controversial results. Thus, this study aimed to assess the effect of sintering temperature on color parameters of zirconia blocks. The null hypothesis was that no significant difference would be found in the translucency parameter of different zirconia types, namely, Ivoclar e. max ZirCAD (IEZ), and White Peaks Symphony (WPS) sintered at different temperatures.
| Materials and Methods|| |
This in vitro experimental study evaluated 30 IEZ (Ivoclar Vivadent, Schaan, Lichtenstein) and 30 WPS (White Peaks Dental De, Germany) zirconia blocks. The sample size was calculated to be 10 in each subgroup according to a previous study. The study was approved by the ethics committee of Hamadan University of Medical Sciences.
IEZ and WPS zirconia specimens measuring 10 mm × 10 mm with 1-mm thickness were milled out of semi-sintered zirconia blocks. Considering 20% shrinkage of zirconia, the specimens were first milled in 12 mm × 12 mm dimensions using a cutting machine (Nemo, Mashhad, Iran). After shrinkage in a furnace, they reached 10 mm × 10 mm dimensions. The specimens in each of the IEZ and WPS groups were randomly divided into three subgroups (n = 10) for sintering at 1440, 1500, and 1530°C. After coloring with A3 shade according to the manufacturers' instructions, the specimens in both zirconia groups were first dried in a furnace (Ceramill Therm, Amann Girrbach, Germany) at 1400°C for 30 min, and then underwent sintering at 1440, 1500, or 1530°C (depending on the assigned subgroup) with a temperature rise of 17°C/min for 2 h.
After sintering, the specimens were placed against a black and a white background and photographed by a digital camera (Canon EOS 6D 20.2MP, 2013, USA). Photography was performed under standard conditions. Daylight was obscured, and two light sources illuminated the specimens at 45° angle. The photographs were transferred to Adobe Photoshop software (Adobe Photoshop CS. Berkeley, CA: Peachpit Press, 2018), the background light was eliminated, and the CIE L* a*b* color parameters were measured., In Photoshop software, the mean L* can range from 0 to 255, while the L* parameter in the CIE system can range from 0 to 100. Thus, the L* parameter was calculated using the formula below: ,,
L* = L × 100/255
Translucency parameter = (L*B-L*W)2+(a*B-a*W)2+
where B indicates the color against a black background and W indicates the color against a white background. L* indicates lightness, a* indicates redness-greenness, and b* indicates yellowness-blueness. The translucency parameter could range from 0 to 100. Lower values indicate lower translucency and vice versa.
Data were analyzed using SPSS version 21 (SPSS Inc., IL, USA). The Kolmogorov–Smirnov test was used to analyze the normality of data distribution. Since the data were normally distributed (P = 0.200), the parametric one-way ANOVA was used to compare translucency among the three subgroups of each zirconia group. Pairwise comparisons of the subgroups were carried out using Tukey's test. The two zirconia groups were compared using one-way ANOVA. P < 0.05 was considered statistically significant.
| Results|| |
[Table 1] shows the mean translucency of the three subgroups of the two zirconia groups. In both IEZ and WPS groups, the maximum and minimum translucency were noted in 1530°C and 1440°C subgroups, respectively. The difference in the mean translucency was significant among the three subgroups of each zirconia group (P = 0.000). Thus, pairwise comparisons of the subgroups within each zirconia group were carried out using Tukey's test. In both zirconia groups, significant differences were noted between every two subgroups such that the mean translucency in 1530°C subgroup was significantly higher than that in 1440°C (P = 0.000) and 1500°C (P = 0.000) subgroups. The mean translucency in 1500°C subgroup was significantly higher than that in 1440°C subgroup (P = 0.000). As shown, in both zirconia groups, increasing the sintering temperature significantly increased the translucency (P = 0.000).
|Table 1: Mean±standard deviation values of translucency parameter of the three subgroups (n=10) of the two zirconia groups|
Click here to view
Comparison of the two zirconia groups revealed that at all three sintering temperatures, the mean translucency of WPS zirconia was significantly higher than that of IEZ zirconia (P < 0.01). The maximum standardized difference between the mean values of the two zirconia groups was observed at 1530°C sintering temperature.
| Discussion|| |
This study assessed the effect of sintering temperatures of 1440°C, 1500°C, and 1530°C on the translucency of IEZ and WPS zirconia blocks. The results showed that the null hypothesis of the study was rejected since significant differences were noted in the translucency of different zirconia blocks sintered at different temperatures. Several factors such as the oxidation rate of stabilizer, distribution of stabilizer, phase composition, size and distribution of particles, and surface treatment affect the quality of zirconia restorations. Despite the independent nature of each of the above-mentioned parameters, they are mainly influenced by the sintering parameters. Zirconia restorations are often sintered at a temperature range of 1350°C–1600°C. Temperatures higher than 1600°C cause excessive growth of particles and increase the porosities. Furthermore, the mechanical and optical properties of zirconia restorations sintered at a temperature lower than 1400°C are not optimal for clinical use.,
In this study, the specimens were photographed against a white background to simulate the clinical setting for posterior teeth and against a black background (for higher light absorption) to simulate the clinical setting for anterior teeth. The L*, a*, and b* color parameters were measured by Photoshop software due to its high accuracy. The results indicated that increasing the sintering temperature in the tested range significantly increased the translucency of both IEZ and WPS zirconia ceramics. Minimum translucency in both groups was noted following sintering at 1440°C, while maximum translucency was recorded following sintering at 1530°C. In line with our findings, many other studies have reported improved translucency of zirconia with different brands as the result of increase in sintering temperature. For instance, Attachoo and Juntavee compared sintering temperatures of 1350°C, 1450°C, and 1550°C and showed that increasing the temperature improved the translucency of zirconia. Sabet et al. compared 1400°C, 1500°C, and 1600°C sintering temperatures with different sintering times and reported maximum translucency after zirconia sintering at 1600°C with minimum sintering time. Sen et al. evaluated sintering of Vita YZ HT and Prettau Zirkonzahn zirconia at 1350°C, 1450°C, and 1600°C temperatures and reported that increasing the sintering temperature significantly increased the translucency. Jiang et al. compared the effects of 1350, 1400, 1450, and 1500°C sintering temperatures on the translucency of zirconia blocks and showed that increasing the sintering temperature significantly increased the density and translucency. Ebeid et al. compared 1460°C, 1530°C, and 1600°C temperatures and reported a reduction in the porosity of zirconia, and subsequently lower light refraction and higher translucency at higher sintering temperatures. Similar results were also reported by many others., Despite the conformity of the above-mentioned results with our findings, it should be noted that these results must be interpreted while taking into account some other important parameters such as the color, strength, and resistance of zirconia, which can also be influenced by the sintering conditions. The reason for our findings is that increasing the temperature or duration of sintering increases the size of zirconia particles, and subsequently, the atomic force between them, which leads to a reduction in micro-porosities in the polycrystalline structure of zirconia. The combined effect of shrinkage of porosities between the particles and accumulation of nanocrystalline zirconia particles results in higher homogeneity of the crystalline structure of zirconia. This leads to light transmission with minimal refractive index, and eventual increase in translucency.,,,, In line with this statement, Gómez et al. showed a reduction in porosity by an increase in temperature such that the relative density increased from 50% to 99%. Furthermore, Sanal and Kilinc demonstrated an increase in size of zirconia particles as the temperature increased from 1350°C to 1450°C and then to 1600°C.
Juntavee and Attashu demonstrated that translucency of Y-TZP zirconia sintered at 1450 and 1550°C was significantly better than that of zirconia sintered at 1350°C. However, the translucency of zirconia sintered at 1450°C was higher than that at 1550°C. Their results were different from our findings, which may be attributed to the difference in methodology and thickness of specimens. In our study, the specimens had 1-mm thickness and they were all sintered for 2 h, while Juntavee and Attashu evaluated specimens with 1.5-mm thickness and variable sintering times. Evidence shows that the thickness of zirconia specimens and duration of sintering affect the zirconia properties. Cardoso et al. found no significant difference in translucency or opacity of zirconia specimens sintered at 1450 and 1600°C; however, light absorption, scattering, and reflectance were significantly different between the two groups. Their results were different from our findings, probably due to the different types of zirconia evaluated in the two studies or the size and thickness of specimens. The specimens in their study were larger and thicker than those in our study.
Zirconia has three phases of cubic, tetragonal, and monoclinic. The monoclinic phase is stable at temperatures up to 1170°C. At higher temperatures, the monoclinic phase gradually transforms to tetragonal, and then to the cubic phase. The translucency of the cubic phase is higher than in other phases. Thus, some authors believe that tetragonal to cubic phase transformation is another reason for increase in translucency. However, the tetragonal to cubic phase transformation at the conventional sintering temperatures is a matter of controversy.,, Öztürk and Can reported that sintering temperature and duration of storage did not affect phase transformation on the surface of zirconia specimens. Ebeid et al. also reported that changing the storage time or sintering temperature did not cause phase transformation in monolithic zirconia, although it increased the translucency. In contrast, Inokoshi et al. evaluated the effect of sintering parameters on phase transformation of three different commercial brands of zirconia and reported an increase in cubic phase on the surface following an increase in sintering temperature and duration of storage of specimens, which led to an increase in translucency. Attachoo and Juntavee confirmed the effect of sintering temperature and duration on the translucency of monolithic zirconia. However, they reported that temperatures higher than 1550°C decreased translucency. They attributed this reduction to an increase in small cracks, which have been reported in some other studies as well., Such small cracks may adversely affect light scattering and consequently the translucency of zirconia blocks.
One limitation of this study was that the zirconia blocks were flat and had no surface complexities; while in the clinical setting, the zirconia crowns have an anatomical shape and complex convex structures. Future studies should be performed on zirconia specimens with a morphology similar to that of tooth morphology to obtain more accurate results. Furthermore, future studies are required to compare the effects of different sintering temperatures on different brands of zirconia and on monolithic versus metal-ceramic restorations.
| Conclusion|| |
Within the limitations of this study, the following conclusions can be drawn:
- Increasing the sintering temperature from 1440°C to 1530°C can significantly increase the translucency of IEZ and WPS zirconia blocks, and can be considered to improve the quality of zirconia restorations
- The mean translucency of WPS zirconia was significantly higher than that of IEZ zirconia.
We would like to express our sincere appreciation to Hamadan University of Medical Sciences for the financial support of this study. (Thesis No. 9805224021 and 9807235417).
Financial support and sponsorship
Conflicts of interest
The authors of this manuscript declare that they have no conflicts of interest, real or perceived, financial or nonfinancial in this article.
| References|| |
Li RW, Chow TW, Matinlinna JP. Ceramic dental biomaterials and CAD/CAM technology: State of the art. J Prosthodont Res 2014;58:208-16.
Petridis HP, Zekeridou A, Malliari M, Tortopidis D, Koidis P. Survival of ceramic veneers made of different materials after a minimum follow-up period of five years: A systematic review and meta-analysis. Eur J Esthet Dent 2012;7:138-52.
Takeichi T, Katsoulis J, Blatz MB. Clinical outcome of single porcelain-fused-to-zirconium dioxide crowns: A systematic review. J Prosthet Dent 2013;110:455-61.
Pieger S, Salman A, Bidra AS. Clinical outcomes of lithium disilicate single crowns and partial fixed dental prostheses: A systematic review. J Prosthet Dent 2014;112:22-30.
Layton DM, Clarke M. A systematic review and meta-analysis of the survival of non-feldspathic porcelain veneers over 5 and 10 years. Int J Prosthodont 2013;26:111-24.
Kelly JR, Benetti P. Ceramic materials in dentistry: Historical evolution and current practice. Aust Dent J 2011;56 Suppl 1:84-96.
Shahmiri R, Standard OC, Hart JN, Sorrell CC. Optical properties of zirconia ceramics for esthetic dental restorations: A systematic review. J Prosthet Dent 2018;119:36-46.
Stawarczyk B, Liebermann A, Eichberger M, Güth JF. Evaluation of mechanical and optical behavior of current esthetic dental restorative CAD/CAM composites. J Mech Behav Biomed Mater 2015;55:1-11.
da Cunha LF, Pedroche LO, Gonzaga CC, Furuse AY. Esthetic, occlusal, and periodontal rehabilitation of anterior teeth with minimum thickness porcelain laminate veneers. J Prosthet Dent 2014;112:1315-8.
Johnston WM. Review of translucency determinations and applications to dental materials. J Esthet Restor Dent 2014;26:217-23.
Vichi A, Louca C, Corciolani G, Ferrari M. Color related to ceramic and zirconia restorations: A review. Dent Mater 2011;27:97-108.
Ryan EA, Tam LE, McComb D. Comparative translucency of esthetic composite resin restorative materials. J Can Dent Assoc 2010;76:a84.
Taruta S, Yamaguchi I, Yamakami T, Yamaguchi T. Sintering behavior and mechanical properties of machinable zirconia/mica composites. J Asian Ceram Soc 2019;7:342-9.
Janney MA, Calhoun CL, Kimrey HD. Microwave sintering of solid oxide fuel cell materials: I, zirconia-8 mol% yttria. J Am Ceram Soc 1992;75:341-6.
Zhang HB, Kim BN, Morita K, Yoshida H, Lim JH, Hiraga K. Optimization of high-pressure sintering of transparent zirconia with nano-sized grains. J Alloy Compd 2010;508:196-9.
Lide DR, editor. CRC Handbook of Chemistry and Physics. Boca Raton, Florida: CRC Press; 2004.
Kelly JR, Nishimura I, Campbell SD. Ceramics in dentistry: Historical roots and current perspectives. J Prosthet Dent 1996;75:18-32.
Anusavice KJ. Recent developments in restorative dental ceramics. J Am Dent Assoc 1993;124:72-4, 76-8, 80-4.
Sen N, Sermet IB, Cinar S. Effect of coloring and sintering on the translucency and biaxial strength of monolithic zirconia. J Prosthet Dent 2018;119:308.e1-7.
Garg SA, Chavda SM. Color masking white fluorotic spots by resin infiltration and its quantitation by computerized photographic analysis: A 12-month follow-up study. Oper Dent 2020;45:1-9.
Heidari A, Shahrabi M, Shahrabi MS. Efficacy of three toothpastes in iron stain removal from primary teeth. Int J Clin Pediatr Dent 2019;12:10-4.
Malek Afzali B, Ghasemi A, Mirani A, Abdolazimi Z, Akbarzade Baghban A, Kharazifard MJ. Effect of ingested liquids on color change of composite resins. J Dent (Tehran) 2015;12:577-84.
Hallmann L, Ulmer P, Reusser E, Louvel M, Hämmerle CH. Effect of dopants and sintering temperature on microstructure and low temperature degradation of dental Y-TZP-zirconia. J Eur Ceram Soc 2012;32:4091-104.
Tinschert J, Natt G, Mautsch W, Augthun M, Spiekermann H. Fracture resistance of lithium disilicate-, alumina-, and zirconia-based three-unit fixed partial dentures: A laboratory study. Int J Prosthodont 2001;14:231-8.
Stawarczyk B, Ozcan M, Hallmann L, Ender A, Mehl A, Hämmerlet CH. The effect of zirconia sintering temperature on flexural strength, grain size, and contrast ratio. Clin Oral Investig 2013;17:269-74.
Jang GW, Kim HS, Choe HC, Son MK. Fracture strength and mechanism of dental ceramic crown with zirconia thickness. Procedia Eng 2011;10:1556-60.
Attachoo S, Juntavee N. Role of sintered temperature and sintering time on spectral translucence of nano-crystal monolithic zirconia. J Clin Exp Dent 2019;11:e146-53.
Sabet H, Wahsh M, Sherif A, Salah T. Effect of different immersion times and sintering temperatures on translucency of monolithic nanocrystalline zirconia. Future Dent J 2018;4:84-9.
Jiang L, Liao Y, Wan Q, Li W. Effects of sintering temperature and particle size on the translucency of zirconium dioxide dental ceramic. J Mater Sci Mater Med 2011;22:2429-35.
Ebeid K, Wille S, Hamdy A, Salah T, El-Etreby A, Kern M. Effect of changes in sintering parameters on monolithic translucent zirconia. Dent Mater 2014;30:e419-24.
Kim MJ, Ahn JS, Kim JH, Kim HY, Kim WC. Effects of the sintering conditions of dental zirconia ceramics on the grain size and translucency. J Adv Prosthodont 2013;5:161-6.
Chen YM, Smales RJ, Yip KH, Sung WJ. Translucency and biaxial flexural strength of four ceramic core materials. Dent Mater 2008;24:1506-11.
Stawarczyk B, Emslander A, Roos M, Sener B, Noack F, Keul C. Zirconia ceramics, their contrast ratio and grain size depending on sintering parameters. Dent Mater J 2014;33:591-8.
Gómez S, Suárez G, Rendtorff NM, Aglietti EF. Relation between mechanical and textural properties of dense materials of tetragonal and cubic zirconia. Sci Sinter 2016;48:119-30.
Sanal FA, Kilinc H. Effect of shade and sintering temperature on the translucency parameter of a novel multi-layered monolithic zirconia in different thicknesses. J Esthet Restor Dent 2020;32:607-14.
Juntavee N, Attashu S. Effect of sintering process on color parameters of nano-sized yttria partially stabilized tetragonal monolithic zirconia. J Clin Exp Dent 2018;10:e794-804.
Kelch M, Schulz J, Edelhoff D, Sener B, Stawarczyk B. Impact of different pretreatments and aging procedures on the flexural strength and phase structure of zirconia ceramics. Dent Mater 2019;35:1439-49.
Cardoso KV, Adabo GL, Mariscal-Muñoz E, Antonio SG, Arioli Filho JN. Effect of sintering temperature on microstructure, flexural strength, and optical properties of a fully stabilized monolithic zirconia. J Prosthet Dent 2020;124:594-8.
Öztürk C, Can G. Effect of sintering parameters on the mechanical properties of monolithic zirconia. J Dent Res Dent Clin Dent Prospects 2019;13:247-52.
Inokoshi M, Zhang F, De Munck J, Minakuchi S, Naert I, Vleugels J, et al.
Influence of sintering conditions on low-temperature degradation of dental zirconia. Dent Mater 2014;30:669-78.
Nogueira AD, Della Bona A. The effect of a coupling medium on color and translucency of CAD-CAM ceramics. J Dent 2013;41 Suppl 3:e18-23.
Della Bona A, Nogueira AD, Pecho OE. Optical properties of CAD-CAM ceramic systems. J Dent 2014;42:1202-9.